Appl Nanosci DOI 10.1007/s13204-017-0552-4
Effects of concentration on CdO films grown by electrodeposition Ayc¸a Kıyak Yıldırım1 • Barıs¸ Altıokka1
Received: 6 February 2017 / Accepted: 2 March 2017 Ó The Author(s) 2017. This article is published with open access at Springerlink.com
Abstract Thin films of CdO were synthesized by electrodeposition via chronoamperometry. The concentrations of aqueous solutions of Cd(NO3)2 were chosen between 0.005 and 0.08 M. It was thought that the reaction rate would reach saturation at 0.02 M of concentration and it was measured as the concentration increased, the thicknesses of the films increased from the 452 nm to the 798 nm. The well-crystallized film was observed to be at 0.01 M of concentration. It was also found that the band gap increased at low concentrations and surface morphology of the films did not change much with concentration. Keywords CdO Electrodeposition Concentration Thin film
At present, CdO films have been prepared by a large range of techniques including molecular beam epitaxy, electrodeposition, sol–gel, sputter deposition, PLD, MOCVD, spray pyrolysis, and activated reactive evaporation (Liu et al. 2012). Among these techniques, electrodeposition is an inherently simple and inexpensive method for preparing semiconductor thin films and has been widely deployed for the preparation of oxide semiconductor thin films (Yogeeswaran et al. 2006). When Cd(NO3)2 is used, the possible formation mechanism of CdO is suggested as follows (Singh et al. 2011a). NO 3 þ H2 O þ 2e ! NO2 þ 2OH
Cd2þ þ 2OH ! CdðOHÞ2
The conversion of Cd(OH)2 to CdO takes place above 280 °C by the following reactions (Singh et al. 2011a). CdðOHÞ2 ! CdO þ H2 O
Transparent oxides have been extensively investigated because of their applications in semiconductor optoelectronic device technology. One of these oxides is cadmium oxide (CdO) (Zialbari and Ghodsi 2011) which is used for optoelectronic applications such as transparent electrodes, solar cells, phototransistors, photodiodes, and gas sensors (Fan 2009). CdO is an n-type semiconductor of a cubic structure with a direct band gap of 2.3 eV (Karim et al. 2016).
In the literature, there are no studies about the effect of concentration on CdO films but there are studies carried out at various concentrations such as 0.025 M (Jayakrishnan and Hodes 2003), 0.02 M (Baykul and Orhan 2014), 0.005 M (Henrı´quez et al. 2010), 0.001 M (Singh et al. 2011b) aqueous solutions of CdCl2, 0.005 M aqueous solution of CdSO4, (Ganjiani et al. 2016), 0.05 M aqueous solution of Cd(C2H3O2)2 (Sarma et al. 2012) and 1 M aqueous solution of Cd(NO3)2 (Singh et al. 2011a).
& Barıs¸ Altıokka [email protected]
Ayc¸a Kıyak Yıldırım [email protected]
In this work, CdO thin films were deposited onto ITOcoated glass substrates using electrodeposition at various concentrations. An Ivium Vertex potentiostat/galvanostat
Bilecik S¸ eyh Edebali University, Bilecik 11210, Turkey
Appl Nanosci Table 1 The deposition conditions in the experiments Experiments
Deposition time (s)
Cathodic potential (V)
71 ± 2
71 ± 2
71 ± 2
71 ± 2
71 ± 2
was used for chronoamperometry method of electrodeposition. Three electrodes which are the reference electrode, the counter electrode (platinum wire) and the working electrode (ITO, 25 X/sq) were used in the experiments. The concentrations were chosen as to be 0.005, 0.01, 0.02, 0.04 and 0.08 M of aqueous solutions of Cd(NO3)2 and named as A1, A2, A3, A4 and A5, respectively. The experiment conditions are given in Table 1. 0.1 M KCl (Potassium Chloride) was used as supporting electrolyte and depositions were completed in 45 min. The deposition temperatures were kept at 72 ± 2 °C using a digital heater and stirrer. After the depositions, the obtained samples were annealed in an oven at 420 °C for Cd(OH)2 turning to CdO. A JASCO V–530 double-beam UV–Vis spectrophotometer was used for analyses of optical properties of the films. The XRD (X-ray diffraction) patterns of the CdO films were obtained by a PANalytical Empyrean X-ray diffractometer. The surface images of the CdO films were
taken by a Zeiss Supra 40VP SEM (scanning electron microscope).
Results and discussion XRD studies of CdO films The current densities versus time plots are given in Fig. 1. The current densities of the films obtained at 0.005 and 0.01 M concentrations demonstrate -0.4 lm/cm2 while the others demonstrate -0.6 lm/cm2 at average. These results show that the reaction rates of the films obtained at 0.005 and 0.01 M are relatively lower than that of the other
Fig. 1 Current density versus time graphs at various molarities of Cd(NO3)2 Table 2 The calculated film thicknesses, crystallite sizes and the optical band gaps Experiments
Crystallite size (nm) Band gap (eV)
Fig. 2 X-ray diffraction pattern of CdO thin films obtained at various molarities of Cd(NO3)2
films. It was concluded that in a previous study (Altıokka 2015), the reaction rate affected thickness, crystallite size, band gap and morphology of the thin films. The film thicknesses of the CdO films were calculated using the gravimetric method and are given in Table 2. As expected, the film thicknesses of the films obtained at 0.005 and 0.01 M are lower than that of the others films. Thicknesses of the films obtained at 0.005 and 0.01 M are average 475 nm while that of the other films are average 790 nm.
The XRD patterns are shown in Fig. 2 and they show the cubic structure of the CdO. There are the two intense diffraction peaks of the CdO located (111) and (002) planes. Although the thicknesses of the films obtained in 0.005 and 0.01 M are thinner than that of the other films, the peak intensities are higher than that of the other films. This shows that the crystallizations of the films obtained at 0.005 and 0.01 M are relatively very good and it also shows that crystallization strongly depends on the reaction rate. The crystallite sizes of the CdO films from the prominent (111) XRD peaks were calculated using Debye– Scherrer formula which is given in Eq. 4. cs ¼
0:089 180 k nm 314 b coshC
where cs is the crystallite size, k is the wavelength of X-ray ˚ ), 2hC is the position of peak center, radiation (1.54056 A and b is the full width at the half maximum of peak height (in degrees) (Bhowmik et al. 2008). The calculated crystallite sizes are given in Table 2. Crystallite sizes are analyzed in Table 2, and it is found that crystallite size depends on reaction rate which is affected by the concentration of the solutions. Optical properties of CdO films Fig. 3 Absorbance spectra of CdO thin films obtained at various molarities of Cd(NO3)2
Absorbances versus wavelength graphs are given in Fig. 3. Absorbance values of the films obtained at 0.005 and
Fig. 4 Plots of (ahm)2 versus hm of CdO thin films for the five different molarities of Cd(NO3)2
0.01 M are lower than that of the other films. It is concluded that film thicknesses and good crystallization cause this result. The absorbance values of the films obtained at 0.02, 0.04 and 0.08 M are nearly same and the thicknesses of these films are also nearly same. This result supports that reaction rate reaches saturation at 0.02 M concentration and this is important because of the fact that there are no works on the reaction rate and the concentration. For estimating the band gaps of the films Tauc plot is used in general. The dependence of a (absorption coefficient) with the photon energy hm can be given by the following equation for the allowed direct transition. 1=2 h ¼ A h Eg ð5Þ where A is the band edge constant and Eg is the optical band gap (Ziabari and Ghodsi 2011; Mkawi et al. 2015; Vishakha et al. 2013). The Eg values were estimated by extrapolating the linear portion of the plots of (ahm)2 vs hm Fig. 5 SEM photographs of the CdO thin films for a 0.005 M, b 0.01 M, c 0.02 M, d 0.04 M and e 0.08 M of Cd(NO3)2
to a = 0 (Ziabari and Ghodsi 2011). For this study, the (ahm)2 vs hm plots are given in Fig. 4 and estimated band gaps of the films are given in Table 2. The band gaps of the films obtained at 0.005 and 0.01 M are 2.63 and 2.59 eV, respectively, whereas the band gap of the bulk CdO is 2.3 eV. It is well known that there is a relation between the band gap and the crystallite size as seen in this work. Due to the fact that concentration affects reaction rate and, therefore, crystallite size, it can be said that there is a relation between the concentration and the band gap. SEM analysis of CdO films SEM photographs were used for analyzing the surface morphology of the CdO films. Figure 5 shows 20,000 magnification SEM images of the CdO thin films. There are no cracks, pinholes or voids on the surfaces of the films and CdO covers the substrate well. It is observed that there are
polymorphic particles on the surfaces. When the concentration of Cd(NO3)2 is increased, the size of these particles is also increased. The surfaces of which are seen in Fig. 5a, b are nearly the same. On the other hand, the surfaces in Fig. 5c, d, e are also nearly the same. These results show that when the reaction rate reaches the saturation, the surfaces do not become different. But when the concentration of Cd(NO3)2 is lower than 0.02 M, filament-like structures appear on the surfaces.
Conclusion In this work, thin films of CdO were deposited by electrodeposition technique onto ITO-coated glass substrates. For the first time, various concentrations such as 0.01, 0.04 and 0.08 M aqueous solutions of Cd(NO3)2 were used and effects of concentration were investigated in detail. It was found out from the current densities and film thicknesses that reaction rate reached the saturation at about 0.02 M of concentration. It was understood from the XRD patterns that good crystallization formed at 0.01 M of concentration. Crystallite sizes of the CdO films were calculated using Debye–Scherrer formula. Below 0.02 M of concentration, the crystallite size decreased from about 60 to 38 nm as the concentration decreased. As a result of this, the optical band gap of the CdO increased up to 2.63 eV. It was clearly seen on the SEM images that CdO covered substrate well and there were no pinholes, voids and cracks. Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http:// creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
References Altıokka A (2015) Effects of inhibitor on PbS thin films obtained by chemical bath deposition. Arab J Sci Eng 40:2085–2093. doi:10. 1007/s13369-015-1680-3 Baykul MC, Orhan N (2014) Effect of seed layer on surface morphological, structural and optical properties of CdO thin
films fabricated by an electrochemical deposition technique. Solid State Electron 101:29–32. doi:10.1016/j.sse.2014.06.033 Bhowmik RN, Nrisimha Murty M, Sekhar Srinadhu E (2008) Magnetic modulation in mechanical alloyed Cr1.4Fe0.6O3 oxide. PMC Phys B 1:20–38. doi:10.1186/1754-0429-1-20 Fan DH (2009) Catalyst-free growth and crystal structures of CdO nanowires and nanotubes. J Cryst Growt 311:2300–2304. doi:10. 1016/j.jcrysgro.2009.01.088 Ganjiani Z, Jamali-Sheini F, Yousefi R (2016) Electrochemical synthesis and physical properties of Sn-doped CdO nanostructures. Superlattice Microst 100:1–9. doi:10.1016/j.spmi.2016.10. 064 Henrı´quez R, Grez P, Mun˜oz E, Go´mez H, Bada´n JA, Marotti RE, Dalchiele EA (2010) Optical properties of CdSe and CdO thin films electrochemically prepared. Thin Solid Films 518:1774–1778. doi:10.1016/j.tsf.2009.09.030 Jayakrishnan R, Hodes G (2003) Non-aqueous electrodeposition of ZnO and CdO films. Thin Solid Films 440:19–25. doi:10.1016/ S0040-6090(03)00811-3 Karim AMMT, Khan MKR, Rahman MM (2016) Effect of Zn/Cd ratio on the optical constants and photoconductive gain of ZnO– CdO crystalline thin films. Mat Sci Semicon Proc 41:184–192. doi:10.1016/j.mssp.2015.08.037 Liu ZQ, Guo R, Li GR, Bu Q, Zhao WX, Tong YX (2012) Facile electrodeposition of large-area CdO and Cd1 - xCoxO curved nanowires. Electrochim Acta 59:449–454. doi:10.1016/j. electacta.2011.10.095 Mkawi EM, Ibrahim K, Ali MKM, Farrukh MA, Mohamed AS (2015) The effect of dopant concentration on properties of transparent conducting Al-doped ZnO thin films for efficient Cu2ZnSnS4 thin-film solar cells prepared by electrodeposition method. Appl Nanosci 5:993–1001. doi:10.1007/s13204-015-0400-3 Sarma B, Smith YR, Mohanty SK, Misra M (2012) Electrochemical deposition of CdO on anodized TiO2 nanotube arrays for enhanced photoelectrochemical properties. Mater Lett 85:33–36. doi:10.1016/j.matlet.2012.06.067 Singh T, Pandya DK, Singh R (2011a) Annealing studies on the structural and optical properties of electrodeposited CdO thin films. Mater Chem Phys 130:1366–1371. doi:10.1016/j. matchemphys.2011.09.035 Singh T, Pandya DK, Singh R (2011b) Electrochemical deposition and characterization of elongated CdO nanostructures. Mater Sci Eng B 176:945–949. doi:10.1016/j.mseb.2011.05.021 Vishakha N, Dhanwate N, Chaure B (2013) Effect of growth potential on the electrodeposition of CIS thin films. Appl Nanosci 3:1–5. doi:10.1007/s13204-012-0063-2 Yogeeswaran G, Chenthamarakshan CR, Seshadri A, de Tacconi NR, Rajeshwar K (2006) Cathodic electrodeposition in the ternary Zn–Cd–O system: mixed (ZnO)x(CdO)1 - x film formation versus Cd-doping of ZnO films. Thin Solif Films 515:2464–2470. doi:10.1016/j.tsf.2006.07.015 Ziabari AA, Ghodsi FE (2011) Optoelectronic studies of sol–gel derived nanostructured CdO–ZnO composite films. J Alloy Compd 509:8748–8755. doi:10.1016/j.jallcom.2011.06.050